#------------------------------------------------------------------------------
#$Date: 2020-10-06 11:03:39 +0200 (mar 06 de oct de 2020) $
#$Revision: 257567 $
#$URL: svn://www.crystallography.net/cod/cif/7/70/51/7705172.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7705172
loop_
_publ_author_name
'Ding, Mengmeng'
'Xu, JingJing'
'Wu, Hongping'
'Yu, Hongwei'
'Hu, Zhanggui'
'Wang, Jiyang'
'Wu, Yicheng'
_publ_section_title
;
 Li₃CaB₂O₅F: a unique sandwich-like
 structure with diverse and wide Li ion diffusion pathways.
;
_journal_issue                   35
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              12184
_journal_page_last               12188
_journal_paper_doi               10.1039/d0dt02423f
_journal_volume                  49
_journal_year                    2020
_chemical_formula_sum            'B4 Ca2 F2 I0 Li6 O10'
_chemical_formula_weight         363.04
_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-03-07 deposited with the CCDC.	2020-08-14 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   25.685(2)
_cell_length_b                   3.4697(3)
_cell_length_c                   5.4404(4)
_cell_measurement_reflns_used    1417
_cell_measurement_temperature    297(2)
_cell_measurement_theta_max      28.52
_cell_measurement_theta_min      3.17
_cell_volume                     484.84(7)
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      297(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0350
_diffrn_reflns_av_unetI/netI     0.0292
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -3
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            2815
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.508
_diffrn_reflns_theta_min         3.173
_exptl_absorpt_coefficient_mu    1.257
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.487
_exptl_crystal_description       bulk
_exptl_crystal_F_000             352
_refine_diff_density_max         0.303
_refine_diff_density_min         -0.454
_refine_diff_density_rms         0.098
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.906
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     79
_refine_ls_number_reflns         656
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.906
_refine_ls_R_factor_all          0.0362
_refine_ls_R_factor_gt           0.0302
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1000P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1009
_refine_ls_wR_factor_ref         0.1104
_reflns_Friedel_coverage         0.000
_reflns_number_gt                577
_reflns_number_total             656
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0dt02423f2.cif
_cod_data_source_block           Li3CaB2O5F
_cod_depositor_comments          'Adding full bibliography for 7705172.cif.'
_cod_database_code               7705172
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ca1 Ca 0.21085(2) 0.750000 0.88690(10) 0.0085(3) Uani 1 2 d S T P . .
Li1 Li 0.1159(2) 0.250000 0.0436(10) 0.0217(13) Uani 1 2 d S T P . .
Li2 Li 0.0316(2) 0.250000 0.4143(10) 0.0230(14) Uani 1 2 d S T P . .
Li3 Li 0.0378(2) 0.750000 0.9324(10) 0.0162(11) Uani 1 2 d S T P . .
B1 B 0.17663(16) 0.250000 0.4022(6) 0.0308(12) Uani 1 2 d S T P . .
B2 B 0.09766(17) -0.1394(13) 0.6189(7) 0.0096(9) Uani 0.5 1 d . . P . .
F1 F 0.03960(7) 0.250000 0.0729(3) 0.0124(4) Uani 1 2 d S T P . .
O2 O 0.20757(7) 0.250000 0.5999(4) 0.0094(5) Uani 1 2 d S T P . .
O3 O 0.11910(8) -0.250000 0.8398(4) 0.0151(5) Uani 1 2 d S T P . .
O4 O 0.19283(8) 0.250000 0.1675(4) 0.0106(5) Uani 1 2 d S T P . .
O5 O 0.04614(8) -0.250000 0.5701(4) 0.0193(6) Uani 1 2 d S T P . .
O6 O 0.12511(10) 0.0436(9) 0.4222(5) 0.0127(7) Uani 0.5 1 d . . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Ca1 O2 95.95(8) 1_565 . ?
O2 Ca1 O4 83.06(5) 1_565 1_566 ?
O2 Ca1 O4 166.60(7) . 1_566 ?
O2 Ca1 O4 166.59(7) 1_565 1_556 ?
O2 Ca1 O4 83.06(5) . 1_556 ?
O4 Ca1 O4 94.80(7) 1_566 1_556 ?
O2 Ca1 O3 83.79(6) 1_565 1_565 ?
O2 Ca1 O3 83.79(6) . 1_565 ?
O4 Ca1 O3 82.81(6) 1_566 1_565 ?
O4 Ca1 O3 82.81(6) 1_556 1_565 ?
O2 Ca1 O2 110.80(4) 1_565 2_565 ?
O2 Ca1 O2 110.80(4) . 2_565 ?
O4 Ca1 O2 81.85(6) 1_566 2_565 ?
O4 Ca1 O2 81.85(6) 1_556 2_565 ?
O3 Ca1 O2 157.27(7) 1_565 2_565 ?
O2 Ca1 O4 75.05(5) 1_565 2_565 ?
O2 Ca1 O4 75.05(5) . 2_565 ?
O4 Ca1 O4 117.28(4) 1_566 2_565 ?
O4 Ca1 O4 117.28(4) 1_556 2_565 ?
O3 Ca1 O4 148.03(7) 1_565 2_565 ?
O2 Ca1 O4 54.70(6) 2_565 2_565 ?
O2 Ca1 B1 93.17(6) 1_565 2_565 ?
O2 Ca1 B1 93.17(6) . 2_565 ?
O4 Ca1 B1 100.23(7) 1_566 2_565 ?
O4 Ca1 B1 100.23(7) 1_556 2_565 ?
O3 Ca1 B1 175.43(9) 1_565 2_565 ?
O2 Ca1 B1 27.30(9) 2_565 2_565 ?
O4 Ca1 B1 27.40(8) 2_565 2_565 ?
O2 Ca1 Li1 124.66(10) 1_565 1_556 ?
O2 Ca1 Li1 74.97(9) . 1_556 ?
O4 Ca1 Li1 94.53(8) 1_566 1_556 ?
O4 Ca1 Li1 42.14(10) 1_556 1_556 ?
O3 Ca1 Li1 41.44(8) 1_565 1_556 ?
O2 Ca1 Li1 123.60(10) 2_565 1_556 ?
O4 Ca1 Li1 145.58(6) 2_565 1_556 ?
B1 Ca1 Li1 140.86(8) 2_565 1_556 ?
O2 Ca1 Li1 74.97(9) 1_565 1_566 ?
O2 Ca1 Li1 124.66(10) . 1_566 ?
O4 Ca1 Li1 42.14(10) 1_566 1_566 ?
O4 Ca1 Li1 94.53(8) 1_556 1_566 ?
O3 Ca1 Li1 41.44(8) 1_565 1_566 ?
O2 Ca1 Li1 123.60(10) 2_565 1_566 ?
O4 Ca1 Li1 145.58(6) 2_565 1_566 ?
B1 Ca1 Li1 140.86(8) 2_565 1_566 ?
Li1 Ca1 Li1 67.74(11) 1_556 1_566 ?
O2 Ca1 B2 75.96(9) 1_565 7_565 ?
O2 Ca1 B2 65.37(9) . 7_565 ?
O4 Ca1 B2 101.56(9) 1_566 7_565 ?
O4 Ca1 B2 91.60(9) 1_556 7_565 ?
O3 Ca1 B2 21.46(8) 1_565 7_565 ?
O2 Ca1 B2 172.89(8) 2_565 7_565 ?
O4 Ca1 B2 127.31(8) 2_565 7_565 ?
B1 Ca1 B2 154.18(10) 2_565 7_565 ?
Li1 Ca1 B2 50.26(13) 1_556 7_565 ?
Li1 Ca1 B2 59.43(12) 1_566 7_565 ?
O2 Ca1 B2 65.37(9) 1_565 1_565 ?
O2 Ca1 B2 75.96(9) . 1_565 ?
O4 Ca1 B2 91.60(9) 1_566 1_565 ?
O4 Ca1 B2 101.56(10) 1_556 1_565 ?
O3 Ca1 B2 21.46(8) 1_565 1_565 ?
O2 Ca1 B2 172.89(8) 2_565 1_565 ?
O4 Ca1 B2 127.31(8) 2_565 1_565 ?
B1 Ca1 B2 154.18(10) 2_565 1_565 ?
Li1 Ca1 B2 59.43(12) 1_556 1_565 ?
Li1 Ca1 B2 50.26(13) 1_566 1_565 ?
B2 Ca1 B2 13.46(16) 7_565 1_565 ?
F1 Li1 O3 94.82(19) . 1_554 ?
F1 Li1 O3 94.83(19) . 1_564 ?
O3 Li1 O3 114.7(3) 1_554 1_564 ?
F1 Li1 O4 156.5(3) . . ?
O3 Li1 O4 97.78(19) 1_554 . ?
O3 Li1 O4 97.78(19) 1_564 . ?
F1 Li1 O6 91.8(2) . . ?
O3 Li1 O6 103.06(12) 1_554 . ?
O3 Li1 O6 140.9(2) 1_564 . ?
O4 Li1 O6 66.07(18) . . ?
F1 Li1 O6 91.8(2) . 7_565 ?
O3 Li1 O6 140.9(2) 1_554 7_565 ?
O3 Li1 O6 103.06(12) 1_564 7_565 ?
O4 Li1 O6 66.07(18) . 7_565 ?
O6 Li1 O6 38.1(2) . 7_565 ?
F1 Li1 B1 124.0(3) . . ?
O3 Li1 B1 113.26(16) 1_554 . ?
O3 Li1 B1 113.26(16) 1_564 . ?
O4 Li1 B1 32.50(12) . . ?
O6 Li1 B1 36.78(14) . . ?
O6 Li1 B1 36.79(14) 7_565 . ?
F1 Li1 B2 84.1(2) . 1_554 ?
O3 Li1 B2 29.63(13) 1_554 1_554 ?
O3 Li1 B2 88.2(2) 1_564 1_554 ?
O4 Li1 B2 115.9(2) . 1_554 ?
O6 Li1 B2 130.91(13) . 1_554 ?
O6 Li1 B2 168.36(19) 7_565 1_554 ?
B1 Li1 B2 140.49(18) . 1_554 ?
F1 Li1 B2 84.1(2) . 7_564 ?
O3 Li1 B2 88.2(2) 1_554 7_564 ?
O3 Li1 B2 29.63(13) 1_564 7_564 ?
O4 Li1 B2 115.9(2) . 7_564 ?
O6 Li1 B2 168.36(19) . 7_564 ?
O6 Li1 B2 130.91(13) 7_565 7_564 ?
B1 Li1 B2 140.49(18) . 7_564 ?
B2 Li1 B2 59.6(2) 1_554 7_564 ?
F1 Li1 Li3 44.22(12) . 1_544 ?
O3 Li1 Li3 51.17(14) 1_554 1_544 ?
O3 Li1 Li3 116.6(3) 1_564 1_544 ?
O4 Li1 Li3 140.31(11) . 1_544 ?
O6 Li1 Li3 94.61(18) . 1_544 ?
O6 Li1 Li3 119.8(3) 7_565 1_544 ?
B1 Li1 Li3 129.36(18) . 1_544 ?
B2 Li1 Li3 50.71(16) 1_554 1_544 ?
B2 Li1 Li3 90.1(2) 7_564 1_544 ?
F1 Li1 Li3 44.22(12) . 1_554 ?
O3 Li1 Li3 116.6(3) 1_554 1_554 ?
O3 Li1 Li3 51.17(14) 1_564 1_554 ?
O4 Li1 Li3 140.31(11) . 1_554 ?
O6 Li1 Li3 119.8(3) . 1_554 ?
O6 Li1 Li3 94.61(18) 7_565 1_554 ?
B1 Li1 Li3 129.36(18) . 1_554 ?
B2 Li1 Li3 90.1(2) 1_554 1_554 ?
B2 Li1 Li3 50.71(16) 7_564 1_554 ?
Li3 Li1 Li3 79.3(2) 1_544 1_554 ?
F1 Li1 Li2 38.33(15) . . ?
O3 Li1 Li2 113.36(17) 1_554 . ?
O3 Li1 Li2 113.36(17) 1_564 . ?
O4 Li1 Li2 118.2(3) . . ?
O6 Li1 Li2 55.87(17) . . ?
O6 Li1 Li2 55.87(17) 7_565 . ?
B1 Li1 Li2 85.7(2) . . ?
B2 Li1 Li2 117.0(2) 1_554 . ?
B2 Li1 Li2 117.0(2) 7_564 . ?
Li3 Li1 Li2 67.20(17) 1_544 . ?
Li3 Li1 Li2 67.20(17) 1_554 . ?
F1 Li2 O5 114.05(18) . 1_565 ?
F1 Li2 O5 114.05(18) . . ?
O5 Li2 O5 123.8(3) 1_565 . ?
F1 Li2 O5 98.7(3) . 5_556 ?
O5 Li2 O5 99.9(2) 1_565 5_556 ?
O5 Li2 O5 99.9(2) . 5_556 ?
F1 Li2 B2 112.2(3) . 7_565 ?
O5 Li2 B2 35.14(15) 1_565 7_565 ?
O5 Li2 B2 99.2(2) . 7_565 ?
O5 Li2 B2 132.5(2) 5_556 7_565 ?
F1 Li2 B2 112.2(3) . . ?
O5 Li2 B2 99.2(2) 1_565 . ?
O5 Li2 B2 35.15(15) . . ?
O5 Li2 B2 132.5(2) 5_556 . ?
B2 Li2 B2 67.3(3) 7_565 . ?
F1 Li2 O6 85.0(2) . 7_565 ?
O5 Li2 O6 63.82(17) 1_565 7_565 ?
O5 Li2 O6 93.6(2) . 7_565 ?
O5 Li2 O6 163.05(9) 5_556 7_565 ?
B2 Li2 O6 33.59(13) 7_565 7_565 ?
B2 Li2 O6 58.92(18) . 7_565 ?
F1 Li2 O6 85.0(2) . . ?
O5 Li2 O6 93.6(2) 1_565 . ?
O5 Li2 O6 63.83(17) . . ?
O5 Li2 O6 163.05(9) 5_556 . ?
B2 Li2 O6 58.93(18) 7_565 . ?
B2 Li2 O6 33.59(13) . . ?
O6 Li2 O6 33.21(16) 7_565 . ?
F1 Li2 Li2 115.6(3) . 5_556 ?
O5 Li2 Li2 124.2(4) 1_565 5_556 ?
O5 Li2 Li2 50.49(11) . 5_556 ?
O5 Li2 Li2 49.4(2) 5_556 5_556 ?
B2 Li2 Li2 130.7(3) 7_565 5_556 ?
B2 Li2 Li2 84.2(2) . 5_556 ?
O6 Li2 Li2 142.9(3) 7_565 5_556 ?
O6 Li2 Li2 114.2(2) . 5_556 ?
F1 Li2 Li2 115.6(3) . 5_566 ?
O5 Li2 Li2 50.49(11) 1_565 5_566 ?
O5 Li2 Li2 124.2(4) . 5_566 ?
O5 Li2 Li2 49.4(2) 5_556 5_566 ?
B2 Li2 Li2 84.2(2) 7_565 5_566 ?
B2 Li2 Li2 130.7(3) . 5_566 ?
O6 Li2 Li2 114.2(2) 7_565 5_566 ?
O6 Li2 Li2 142.9(3) . 5_566 ?
Li2 Li2 Li2 85.6(4) 5_556 5_566 ?
F1 Li2 Li3 49.69(19) . 5_566 ?
O5 Li2 Li3 116.32(17) 1_565 5_566 ?
O5 Li2 Li3 116.32(17) . 5_566 ?
O5 Li2 Li3 49.04(18) 5_556 5_566 ?
B2 Li2 Li3 144.08(15) 7_565 5_566 ?
B2 Li2 Li3 144.08(15) . 5_566 ?
O6 Li2 Li3 132.1(2) 7_565 5_566 ?
O6 Li2 Li3 132.1(2) . 5_566 ?
Li2 Li2 Li3 80.1(3) 5_556 5_566 ?
Li2 Li2 Li3 80.1(3) 5_566 5_566 ?
F1 Li2 Li1 40.71(18) . . ?
O5 Li2 Li1 98.9(2) 1_565 . ?
O5 Li2 Li1 98.9(2) . . ?
O5 Li2 Li1 139.4(3) 5_556 . ?
B2 Li2 Li1 78.6(2) 7_565 . ?
B2 Li2 Li1 78.6(2) . . ?
O6 Li2 Li1 46.44(15) 7_565 . ?
O6 Li2 Li1 46.44(15) . . ?
Li2 Li2 Li1 135.59(19) 5_556 . ?
Li2 Li2 Li1 135.59(19) 5_566 . ?
Li3 Li2 Li1 90.4(2) 5_566 . ?
F1 Li3 F1 132.4(3) 1_566 1_556 ?
F1 Li3 O5 113.46(16) 1_566 1_565 ?
F1 Li3 O5 113.46(16) 1_556 1_565 ?
F1 Li3 F1 91.73(19) 1_566 5_566 ?
F1 Li3 F1 91.73(19) 1_556 5_566 ?
O5 Li3 F1 95.4(3) 1_565 5_566 ?
F1 Li3 O3 94.07(19) 1_566 1_565 ?
F1 Li3 O3 94.07(19) 1_556 1_565 ?
O5 Li3 O3 70.2(2) 1_565 1_565 ?
F1 Li3 O3 165.6(3) 5_566 1_565 ?
F1 Li3 B2 115.5(2) 1_566 7_565 ?
F1 Li3 B2 97.38(19) 1_556 7_565 ?
O5 Li3 B2 36.90(16) 1_565 7_565 ?
F1 Li3 B2 130.5(3) 5_566 7_565 ?
O3 Li3 B2 35.53(14) 1_565 7_565 ?
F1 Li3 B2 97.38(19) 1_566 1_565 ?
F1 Li3 B2 115.5(2) 1_556 1_565 ?
O5 Li3 B2 36.90(16) 1_565 1_565 ?
F1 Li3 B2 130.5(3) 5_566 1_565 ?
O3 Li3 B2 35.53(14) 1_565 1_565 ?
B2 Li3 B2 19.0(2) 7_565 1_565 ?
F1 Li3 Li2 108.04(18) 1_566 5_566 ?
F1 Li3 Li2 108.04(18) 1_556 5_566 ?
O5 Li3 Li2 49.6(2) 1_565 5_566 ?
F1 Li3 Li2 45.77(18) 5_566 5_566 ?
O3 Li3 Li2 119.8(3) 1_565 5_566 ?
B2 Li3 Li2 85.5(3) 7_565 5_566 ?
B2 Li3 Li2 85.5(3) 1_565 5_566 ?
F1 Li3 Li3 119.6(3) 1_566 5_567 ?
F1 Li3 Li3 47.27(9) 1_556 5_567 ?
O5 Li3 Li3 110.3(3) 1_565 5_567 ?
F1 Li3 Li3 44.46(17) 5_566 5_567 ?
O3 Li3 Li3 139.59(16) 1_565 5_567 ?
B2 Li3 Li3 124.6(2) 7_565 5_567 ?
B2 Li3 Li3 141.1(3) 1_565 5_567 ?
Li2 Li3 Li3 72.8(2) 5_566 5_567 ?
F1 Li3 Li3 47.27(8) 1_566 5_577 ?
F1 Li3 Li3 119.6(3) 1_556 5_577 ?
O5 Li3 Li3 110.3(3) 1_565 5_577 ?
F1 Li3 Li3 44.46(17) 5_566 5_577 ?
O3 Li3 Li3 139.59(16) 1_565 5_577 ?
B2 Li3 Li3 141.1(3) 7_565 5_577 ?
B2 Li3 Li3 124.6(2) 1_565 5_577 ?
Li2 Li3 Li3 72.8(2) 5_566 5_577 ?
Li3 Li3 Li3 79.7(3) 5_567 5_577 ?
F1 Li3 Li1 46.27(14) 1_566 1_566 ?
F1 Li3 Li1 118.4(3) 1_556 1_566 ?
O5 Li3 Li1 98.1(2) 1_565 1_566 ?
F1 Li3 Li1 137.76(13) 5_566 1_566 ?
O3 Li3 Li1 48.36(14) 1_565 1_566 ?
B2 Li3 Li1 77.4(2) 7_565 1_566 ?
B2 Li3 Li1 64.6(2) 1_565 1_566 ?
Li2 Li3 Li1 131.91(18) 5_566 1_566 ?
Li3 Li3 Li1 151.4(3) 5_567 1_566 ?
Li3 Li3 Li1 93.42(15) 5_577 1_566 ?
F1 Li3 Li1 118.4(3) 1_566 1_556 ?
F1 Li3 Li1 46.27(14) 1_556 1_556 ?
O5 Li3 Li1 98.1(2) 1_565 1_556 ?
F1 Li3 Li1 137.76(13) 5_566 1_556 ?
O3 Li3 Li1 48.36(14) 1_565 1_556 ?
B2 Li3 Li1 64.6(2) 7_565 1_556 ?
B2 Li3 Li1 77.4(2) 1_565 1_556 ?
Li2 Li3 Li1 131.91(18) 5_566 1_556 ?
Li3 Li3 Li1 93.42(15) 5_567 1_556 ?
Li3 Li3 Li1 151.4(3) 5_577 1_556 ?
Li1 Li3 Li1 79.3(2) 1_566 1_556 ?
O2 B1 O4 125.5(3) . . ?
O2 B1 O6 117.6(3) . . ?
O4 B1 O6 109.9(3) . . ?
O2 B1 O6 117.6(3) . 7_565 ?
O4 B1 O6 109.9(3) . 7_565 ?
O6 B1 O6 56.7(3) . 7_565 ?
O2 B1 Li1 177.8(3) . . ?
O4 B1 Li1 56.7(2) . . ?
O6 B1 Li1 60.56(19) . . ?
O6 B1 Li1 60.56(19) 7_565 . ?
O2 B1 Ca1 55.20(16) . 2_564 ?
O4 B1 Ca1 70.29(19) . 2_564 ?
O6 B1 Ca1 151.50(14) . 2_564 ?
O6 B1 Ca1 151.51(14) 7_565 2_564 ?
Li1 B1 Ca1 127.02(18) . 2_564 ?
O2 B1 Ca1 36.22(7) . . ?
O4 B1 Ca1 133.00(17) . . ?
O6 B1 Ca1 115.4(2) . . ?
O6 B1 Ca1 85.74(15) 7_565 . ?
Li1 B1 Ca1 142.75(10) . . ?
Ca1 B1 Ca1 75.82(8) 2_564 . ?
O2 B1 Ca1 36.22(7) . 1_545 ?
O4 B1 Ca1 133.00(17) . 1_545 ?
O6 B1 Ca1 85.74(15) . 1_545 ?
O6 B1 Ca1 115.4(2) 7_565 1_545 ?
Li1 B1 Ca1 142.75(10) . 1_545 ?
Ca1 B1 Ca1 75.82(8) 2_564 1_545 ?
Ca1 B1 Ca1 63.94(7) . 1_545 ?
B2 B2 O3 73.81(19) 7 . ?
B2 B2 O5 74.12(19) 7 . ?
O3 B2 O5 117.8(3) . . ?
B2 B2 O6 116.4(2) 7 . ?
O3 B2 O6 125.4(3) . . ?
O5 B2 O6 116.4(3) . . ?
B2 B2 O6 42.42(15) 7 7 ?
O3 B2 O6 97.9(3) . 7 ?
O5 B2 O6 92.4(2) . 7 ?
O6 B2 O6 73.9(3) . 7 ?
B2 B2 Li3 80.51(12) 7 1_545 ?
O3 B2 Li3 65.1(2) . 1_545 ?
O5 B2 Li3 58.1(2) . 1_545 ?
O6 B2 Li3 161.3(3) . 1_545 ?
O6 B2 Li3 122.4(2) 7 1_545 ?
B2 B2 Li2 123.66(13) 7 . ?
O3 B2 Li2 146.3(3) . . ?
O5 B2 Li2 53.77(17) . . ?
O6 B2 Li2 75.8(2) . . ?
O6 B2 Li2 114.2(2) 7 . ?
Li3 B2 Li2 88.1(2) 1_545 . ?
B2 B2 Li1 119.82(11) 7 1_556 ?
O3 B2 Li1 47.74(16) . 1_556 ?
O5 B2 Li1 117.3(3) . 1_556 ?
O6 B2 Li1 109.3(3) . 1_556 ?
O6 B2 Li1 141.5(2) 7 1_556 ?
Li3 B2 Li1 64.69(17) 1_545 1_556 ?
Li2 B2 Li1 103.4(2) . 1_556 ?
B2 B2 Ca1 83.28(8) 7 1_545 ?
O3 B2 Ca1 39.05(16) . 1_545 ?
O5 B2 Ca1 152.8(3) . 1_545 ?
O6 B2 Ca1 87.0(2) . 1_545 ?
O6 B2 Ca1 80.49(16) 7 1_545 ?
Li3 B2 Ca1 103.92(18) 1_545 1_545 ?
Li2 B2 Ca1 152.4(2) . 1_545 ?
Li1 B2 Ca1 61.77(13) 1_556 1_545 ?
Li2 F1 Li3 113.45(16) . 1_544 ?
Li2 F1 Li3 113.45(16) . 1_554 ?
Li3 F1 Li3 132.4(3) 1_544 1_554 ?
Li2 F1 Li1 101.0(3) . . ?
Li3 F1 Li1 89.51(19) 1_544 . ?
Li3 F1 Li1 89.51(19) 1_554 . ?
Li2 F1 Li3 84.5(3) . 5_566 ?
Li3 F1 Li3 88.27(19) 1_544 5_566 ?
Li3 F1 Li3 88.27(19) 1_554 5_566 ?
Li1 F1 Li3 174.5(2) . 5_566 ?
B1 O2 Ca1 124.00(9) . . ?
B1 O2 Ca1 124.00(9) . 1_545 ?
Ca1 O2 Ca1 95.95(8) . 1_545 ?
B1 O2 Ca1 97.5(2) . 2_564 ?
Ca1 O2 Ca1 106.98(6) . 2_564 ?
Ca1 O2 Ca1 106.98(6) 1_545 2_564 ?
B2 O3 B2 32.4(4) . 7 ?
B2 O3 Li1 102.6(2) . 1_556 ?
B2 O3 Li1 133.5(3) 7 1_556 ?
B2 O3 Li1 133.5(3) . 1_546 ?
B2 O3 Li1 102.6(2) 7 1_546 ?
Li1 O3 Li1 114.7(3) 1_556 1_546 ?
B2 O3 Li3 79.4(2) . 1_545 ?
B2 O3 Li3 79.4(2) 7 1_545 ?
Li1 O3 Li3 80.46(18) 1_556 1_545 ?
Li1 O3 Li3 80.46(18) 1_546 1_545 ?
B2 O3 Ca1 119.5(2) . 1_545 ?
B2 O3 Ca1 119.5(2) 7 1_545 ?
Li1 O3 Ca1 88.97(16) 1_556 1_545 ?
Li1 O3 Ca1 88.97(16) 1_546 1_545 ?
Li3 O3 Ca1 160.21(18) 1_545 1_545 ?
B1 O4 Li1 90.8(3) . . ?
B1 O4 Ca1 132.59(4) . 1_544 ?
Li1 O4 Ca1 88.66(12) . 1_544 ?
B1 O4 Ca1 132.59(4) . 1_554 ?
Li1 O4 Ca1 88.66(12) . 1_554 ?
Ca1 O4 Ca1 94.80(7) 1_544 1_554 ?
B1 O4 Ca1 82.3(2) . 2_564 ?
Li1 O4 Ca1 173.08(18) . 2_564 ?
Ca1 O4 Ca1 96.01(6) 1_544 2_564 ?
Ca1 O4 Ca1 96.01(6) 1_554 2_564 ?
B2 O5 B2 31.7(4) 7 . ?
B2 O5 Li2 120.1(3) 7 . ?
B2 O5 Li2 91.1(2) . . ?
B2 O5 Li2 91.1(2) 7 1_545 ?
B2 O5 Li2 120.1(3) . 1_545 ?
Li2 O5 Li2 123.8(3) . 1_545 ?
B2 O5 Li3 85.0(3) 7 1_545 ?
B2 O5 Li3 85.0(3) . 1_545 ?
Li2 O5 Li3 114.08(17) . 1_545 ?
Li2 O5 Li3 114.08(17) 1_545 1_545 ?
B2 O5 Li2 159.1(2) 7 5_556 ?
B2 O5 Li2 159.1(2) . 5_556 ?
Li2 O5 Li2 80.1(2) . 5_556 ?
Li2 O5 Li2 80.1(2) 1_545 5_556 ?
Li3 O5 Li2 81.4(2) 1_545 5_556 ?
B2 O6 O6 116.4(2) . 7_565 ?
B2 O6 B1 134.2(3) . . ?
O6 O6 B1 61.66(14) 7_565 . ?
B2 O6 B2 21.2(3) . 7 ?
O6 O6 B2 137.58(15) 7_565 7 ?
B1 O6 B2 135.8(3) . 7 ?
B2 O6 Li1 142.6(3) . . ?
O6 O6 Li1 70.95(10) 7_565 . ?
B1 O6 Li1 82.7(2) . . ?
B2 O6 Li1 136.9(2) 7 . ?
B2 O6 Li2 70.6(2) . . ?
O6 O6 Li2 73.39(8) 7_565 . ?
B1 O6 Li2 134.7(2) . . ?
B2 O6 Li2 82.24(18) 7 . ?
Li1 O6 Li2 77.69(19) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ca1 O2 2.3354(14) 1_565 ?
Ca1 O2 2.3354(14) . ?
Ca1 O4 2.3568(13) 1_566 ?
Ca1 O4 2.3568(13) 1_556 ?
Ca1 O3 2.370(2) 1_565 ?
Ca1 O2 2.395(2) 2_565 ?
Ca1 O4 2.747(2) 2_565 ?
Ca1 B1 2.891(4) 2_565 ?
Ca1 Li1 3.113(4) 1_556 ?
Ca1 Li1 3.113(4) 1_566 ?
Ca1 B2 3.275(4) 7_565 ?
Ca1 B2 3.275(4) 1_565 ?
Li1 F1 1.965(6) . ?
Li1 O3 2.061(3) 1_554 ?
Li1 O3 2.061(3) 1_564 ?
Li1 O4 2.089(6) . ?
Li1 O6 2.194(6) . ?
Li1 O6 2.194(6) 7_565 ?
Li1 B1 2.498(7) . ?
Li1 B2 2.717(7) 1_554 ?
Li1 B2 2.717(7) 7_564 ?
Li1 Li3 2.719(6) 1_544 ?
Li1 Li3 2.719(6) 1_554 ?
Li1 Li2 2.958(8) . ?
Li2 F1 1.869(6) . ?
Li2 O5 1.966(3) 1_565 ?
Li2 O5 1.966(3) . ?
Li2 O5 1.999(6) 5_556 ?
Li2 B2 2.437(6) 7_565 ?
Li2 B2 2.437(6) . ?
Li2 O6 2.506(6) 7_565 ?
Li2 O6 2.506(6) . ?
Li2 Li2 2.553(9) 5_556 ?
Li2 Li2 2.553(9) 5_566 ?
Li2 Li3 2.596(8) 5_566 ?
Li3 F1 1.896(2) 1_566 ?
Li3 F1 1.896(2) 1_556 ?
Li3 O5 1.983(6) 1_565 ?
Li3 F1 1.989(6) 5_566 ?
Li3 O3 2.148(6) 1_565 ?
Li3 B2 2.328(7) 7_565 ?
Li3 B2 2.328(7) 1_565 ?
Li3 Li3 2.706(8) 5_567 ?
Li3 Li3 2.706(8) 5_577 ?
B1 O2 1.338(4) . ?
B1 O4 1.343(4) . ?
B1 O6 1.508(4) . ?
B1 O6 1.509(4) 7_565 ?
B2 B2 0.768(9) 7 ?
B2 O3 1.376(4) . ?
B2 O5 1.403(5) . ?
B2 O6 1.430(5) . ?
B2 O6 1.900(5) 7 ?
O6 O6 1.432(7) 7_565 ?
